Crumb Rubber Modified Asphalt Concrete for Low Noise ?· Crumb Rubber Modified Asphalt Concrete for…
Post on 05-Jun-2018
Embed Size (px)
Information about research of the paper
Information about research of the paper
Crumb Rubber Modified Asphalt Concretefor Low Noise Surfaces
Massimo Losa, Pietro Leandri, Patrizia Rocchio
University of Pisa, Department of Civil Engineering (DIC)Largo Lucio Lazzarino, 1 56122 Pisa (Italy)
firstname.lastname@example.org, email@example.com, firstname.lastname@example.org
ABSTRACT. The principal advantage of introducing some percentages of crumb rubber inproduction of asphalt mixtures is related to pavement environmental sustainability, since thisprocess allows to recycle a significant amount of an industrial waste and, in some specificcases, to reduce tire/road noise emissions; there are some other not unanimously recognizedadvantages related to this process that are the improvement of asphalt mixture mechanicalproperties and durability as well as friction on pavement surface. This paper reports on aresearch project carried out to evaluate the advantages of using crumb rubber inconstruction of low noise gap graded asphalt concrete surfaces, specifically designed toreduce rolling noise by optimizing surface texture. The study also aimed to define themechanical and functional performances of the mix obtained by using the wet process inorder to assess its potential for use as viable alternative to other low noise asphalt surfacesaimed to improve pavement sustainability by reducing environmental, social and economicimpacts. Results of laboratory and on site tests, carried out on one specifically built fieldtrial, clearly show this mix can have optimal mechanical and functional performance as wellas it can reduce tire/road noise and warrant greater durability of wearing layers; thisconsidering, crumb rubber modified asphalt concrete can be classified as a constructionmaterial that can enhance the three dimensions of sustainability.
KEYWORDS: environmental sustainability, low noise asphalt surface, wet process, crumbrubber, pavement sustainability
2 Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces
Scrap tires form a major part of the worlds solid waste management problem;in addition, market groups forecast that in the next years post consumer tires willincrease. At the same time, the increasing demand for road transportation hascaused serious problems of noise pollution due to vehicular traffic.
These are only two of the problems resulting from the continuous increase intransportation demand, which has prompted the international scientific communityto search for innovative solutions that allow to use crumb rubber tire in asphaltpavements.
The advantage of using crumb rubber in the production of asphalt mixtures isnot limited to the improvement of road sustainability, but it can be related to animprovement of mechanical properties or a reduction of noise emissions, inaddition an increase of friction (,  and ). At the present time, theinternational scientific community is not unanimous in judging the positive effectsof crumb rubber in terms of reduction of noise emission. According to Sandbergand Ejsmont  there is no evidence that the insertion of small quantities of crumbrubber within asphalt mixtures can allow to significantly reduce tire/road noise.
The use of crumb rubber in asphalt pavements dates back to many years ago (and ). In the Wet process, crumb rubber and bitumen are mixed and left to reactat high temperatures: the final result is known as Asphalt Rubber (AR) (, and ). The AR is used as a modified bitumen in the production of porous asphaltconcretes (open graded) and gap graded asphalt concretes characterized by binderpercentages ranging between 7 and 9%, to which corresponds a crumb rubberpercentage of 1 1.5% on the mixture weight. Moreover, for the need of allowingthe reaction between bitumen and crumb rubber (,  and ), in the Wetprocess it is necessary to use specific mixers for production of the modified asphaltat high temperatures.
This paper reports on research conducted to evaluate the feasibility of using ARin the construction of low noise gap graded asphalt surfaces. The study also aimedto define the mechanical and functional performances of the resulting mix in orderto assess its potential for use as a viable alternative, in terms of environmentalcompatibility and costs, to low noise open-graded asphalt surface. This mix allowsoptimal mechanical and functional performance, it reduces tire road noise andguarantees greater durability of wearing layer performance; in addition, it isenvironmentally friend, by offering a better life-cycle assessment for scrap tire.
Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces 3
2. Use of crumb rubber modifier in asphalt mixes
The material widely used in vehicle tires is Styrene-Butadiene-Rubber (SBR)that is a synthetic rubber copolymer consisting of styrene and butadiene. It hasgood abrasion resistance and good aging stability when protected by additives;crumb rubber used in this study comes from mechanical grinding of scrap tires atroom temperature; they are represented by 50% by weight of truck tires and 50%by weight of car tires. Figure 1 represents size gradation of crumb rubber used toproduce gap graded mix, according to the wet processes, overlaid to the typicalCRM gradations for production of the Asphalt Rubber. The size gradation of crumbrubber fulfils the requirements of CRM for the production of Asphalt Rubber .
0.01 0.10 1.00 10.00
Sieve size [mm]
Typical Gradation -CRM for AR
Figure 1. The size gradation of crumb rubber
3. Description of experiment
The experiment involved a first step of mix design to define the aggregate grainsize distributions and the optimum asphalt contents to be used in the mix; in thesecond step, laboratory tests were carried out to evaluate mixture performance.
The gap graded asphalt mixture produced by the wet process, was utilized for asurface layer, 3 cm thick, laid on a roughly 150 m long test section within theLeopoldo research project . This project has the specific aim of improvingroad safety and environmental compatibility.
Cores were taken from pavement to check the compliance with the designmixture in terms of aggregate gradation, asphalt content and air void percentage.The in-situ characteristics of the mixture was substantially the same of thelaboratory mixture with regard to the aggregate gradation and the bitumen content;
4 Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces
as far as the air void contents of in situ mixture, they were approximately 2% morethan the air void contents of the laboratory mixture.
This asphalt wearing course was then evaluated in terms of surfacecharacteristics (friction and texture) and acoustic performance.
4. Mix design
Mix design was carried out by the volumetric method. The optimum asphaltcontent was identified by optimizing the air void contents.
4.1. Aggregate gradation
Physical properties of aggregates, determined according to the UNI-EN 1097-6/7 procedures, are shown in Table 1.
Physical proprieties Basalt 4/6 Sand Mineral Filler
Bulk Specific Gravity
(kg/m3)2753 2629 2650
Apparent Specific Gravity
(kg/m3)2863 2690 2650
(%)1.39 0.86 0.00
Table 1. Asphalt binders characteristics
Sieve size [mm - raised to 0.45 power]
5 2 4
Figure 2. Aggregate size gradation
Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces 5
The grain size distribution of the studied mixture respects the aggregategradation required by the project specifications for gap graded asphalt mixtureswith the maximum aggregate size equals to 8.0 mm (Figure 2).
The resulting internal structure of the mixture determined by the discontinuousaggregate grading curve can be appreciated in Figure 3.
Figure 3. Internal structure of the mixes
4.2. Optimum asphalt content and volumetric properties of the mixture
The aggregates were mixed with Asphalt Rubber (AR) (Table 2), consisting of20% CRM by weight of binder and the remaining 80% of 50-70 penetration gradebitumen. The optimum asphalt content of the mix was determined by gyratorycompaction, assessing the volumetric characteristics of four mixtures with asphaltcontents ranging from 7.5% to 9.0% (Table 3).
In determining the volumetric properties of the mixes, the aggregate absorptionpercentage was assumed to be equal to 1/3 of water absorption, as required by UNIEN 12697-5.
From the mix design it is possible to determine the optimum percentage ofbitumen capable of minimizing the void percentage and guaranteeing at thecompaction level Nmax a void volume higher than 2% and at the compaction levelNdesign a void volume ranging between 3 5%. From the results obtained it wasselected the optimum bitumen content equal to 8.5%.
6 Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces
Unit Value Reference
Penetration at 25 C Dmm 25 55 UNI EN 1426
Softening point, Ring & Ball C 58 UNI EN 1427
Fraass breaking point C -7 UNI EN 12593
Flash Point C 250 EN ISO 2592
Elastic recovery at 25 C % 70 UNI EN 13398
Resistance to hardening RTFOT (163 C UNI EN 12607-1)
Loss in mass % 0.5